Paint Additive Evaluation and Characterization

=Problem Definition=
Our goal is to evaluate the thermal resistance, solar heat reflectance, and microstructure durability of two novel paint additive technologies.
==Background==
Many paint additives have started being tested in many various applications. There have been multiple tests that show that these additives can have some benefits to thermal resistivity, temperature reduction, and some degree of EMF protection. There are two main types of different paint additives that have been tested the first being a nano-ceramic additive and the second being a phase change additive. Both of these additives modify the thermal conductivity (k) and the emissivity (Ɛ) of the base paint. These help to reduce the heat absorption rate from radiated and latent heat. In addition to the beneficial properties, these additives are relatively cheap when compared to the price of a coating system. if a temperature drop could be observed under strenuous testing in a variety of environments and meet paint coating test specifications it could be a great cost per benefit solution to reflect heat and reduce internal temperatures.
==Deliverables==
The addition of these paint additives must show the following:
* Show a temperature reduction of 5 degrees Fahrenheit in warm weather
* Increase thermal resistivity to provide insulation and an increase from the ambient temperature of 5 degrees
* Meet Salt fog testing (ASTM B117) Requirements for 1500 hours of testing ​
* Meet Mean Creepback Rating (ASTM D1654, Procedure A) for 1500 hours of testing 
==Value Proposistion Statement==
The lifetime of electronic devices, found inside enclosures, is significantly shortened when exposed to environmental extremes. Because there are thousands of enclosures in rural locations, hot and cold climates, it is essential to develop an affordable, maintenance-free method to extend the life of the enclosure’s internal electronic devices. By using affordable paint additive technologies any improvement in performance and extension of application life will be financially beneficial for the client. The Nano-Vandalizers are offering an affordable, simple solution to reduce the thermal degradation of electrical enclosures in order to extend the battery life and reduce the possibilities of a short circuit due to a buildup of condensation. We will coat SEL’s enclosures with the paint additive technologies to evaluate the thermal resistance, solar heat reflectance, and microstructure durability of the enclosure surface.
=Design Considerations=
==Testing Stand Design==
A test stand had to be designed to create a uniform and consistent testing environment to achieve the best results from temperature and resistivity testing. In addition to these requirements. The test stands also had to be designed to assemble quickly and take up a minimum amount of room. The test stand was designed to be mounted on a 4' by 4' piece of plywood with a 4" by 4" stand to mount the cabinets with a large lag screw. The 4" by 4" is supported by three 2"x4" struts cut at a 45-degree angle and fastened to the plywood.
File:NVSTANDFRONT.jpg|front view
File:NVSTANDSIDE.jpg|side view
File:NVSTANDISO.jpg|Isometric view
===Revisions to the test stand===
After consulting with the party that was going to house our enclosures and monitor our testing, It was then made clear that our stand had to revise for space and assembly considerations. The design was kept very similar but the sizes of the 2x4 struts and plywood were revised. It was decided to cut the 2x4 struts to an equal length due to the relatively light load of the cabinet being supported. The plywood was decided to be cut to a 28 by 28 square footprint rather than the previously 4' by 4' footprint. The two by fours were then decided to be cut to even lengths of 30" rather than having two sizes of 2x4 cuts. The revised views can be seen below
File:NVREVISEDSTAND3VIEW.jpg|final testing view
File:NVREVISEDSTANDISO.jpg|Isometric view
===Final Test Stand Images===
Our test stands were assembled on November 11th of 2020 in the design suite. 
File:NVASSEMBLEDSTANDREAL.jpg|Final Assembly of The testing stands
=Thermal Testing procedures=
==Thermal resistivity Testing==
In order to create thermal resistivity models, the thermal conductivity constant (k) of each coating had to be found. These values are found by using Fourier's law in one dimension :
\phi_\text{q} = -k \frac{dT(x)}{dx}
With (k) being the thermal conductivity factor, \phi_\text{q} representing the heat flux across the surface and \frac{dT(x)}{dx} representing the temperature gradient across the surface. To measure the heat flux across the entire surface of the cabinets we will be calculated by first finding the thermal conductivity of the control cabinet. after this is completed, then the heat flux across the surface can be found by the use of a temperature sensor positioned on the inner and outer surface of the cabinet. With these values calculated the heat flux across the surface from convective and conductive heat transfer can be calculated. With this information, the thermal conductivity of each paint coating with its respective additive can be quantified
==Energy consumption Testing==
===Heater Circuit===
To satisfy the project requirement for insulative properties we found it necessary to create a heater circuit. with this circuit, we could test how much energy is being used to keep the enclosure at a constant heat. in addition, we can show the temperature differences with our temperature sensors
====Heater circuit methods and parts====
To construct the heater circuit, we used an Arduino Uno microcontroller along with a MAX6675 thermocouple amplifier with a K-type thermocouple which allows for accurate temperature readings. to control the heater side, we used a solid-state relay which allows for us to control when the circuit comes on. In addition, we also timed how long the circuit was active for which can give us a direct comparison of the energy use between the two enclosures. 
File:Initialcircuitdesign.png|Heater Circuit Schematic
File:Pricing.jpg|Pricing for heater circuit components
===Testing Apparatus and setup===
To evaluate the phase change coating Our team mixed it with a Sherman Williams house paint as it was incompatible with the oil-based coatings that were used on the Cabinets. Our team picked two enclosures and painted one with a control coating and the other with the phase change material embedded in the coating. These enclosures were also sealed with expansion foam and weatherstripping to seal the enclosures and provide the best data. The apparatus and enclosures can be seen in the images below:
20210425_093940.jpg|side by side enclosures
20210402 155300.jpg|heater in enclosures
==Temperature Sensor Placement and outdoor data collection==
In the electronics that are placed inside of these containers, There is a battery that powers the previously mentioned electronics. This component is one of the most susceptible to damage from extreme temperatures and extreme temperature fluctuations. In the cabinets, the battery is placed in the bottom right of the enclosure. Because of this, the sensors were placed on the front door of the cabinet, the bottom of the cabinet, and on the inside of the cabinet near the bottom of the enclosure. these locations allowed us to have temperature information where it is most important to the supplier. The types of Sensors that will be used to collect data are called HOBO sensors and can be seen below.
File:NVHOBOSENSORWSENSOR.jpg|Hobo Sensor with additional sensor
File:NVHOBOMOUNTING.jpg|Hobo Sensor Mounting 
File:NVHOBOMOUNTINWENCLOSURE.jpg|150x150px|Simulation of Sensor in the cabinet
These sensors can have an additional temperature probe plugged into a socket into the base sensor to procure two temperature data measurements from two different locations. The sensors will be mounted to the cabinets with the use of velcro. The temperature data will be collected every 15 minutes and will be taken from the sensor every month. An example of the Sensor placement can be seen below with a painted cabinet
File:Cabinet in actuality.jpg|Sensor placed in the coated cabinet
=Paint durability tests=
==Salt Fog Testing==
One test that SEL conducts to characterize the durability of their paint coating is a salt fog test. In addition to characterizing the durability of the paint coatings, it can also help characterize the corrosion resistance of a paint coating. In order for these paint additives to be implemented into SEL's existing paint process, each respective coating must be able to protect the base metal underneath the cabinets to a certain standard that meets or exceeds the current paint coating. These Standards are as follows: MEK Test (ASTM D4752-03), Cross-Hatch Adhesion Test (ASTM D3539), Salt Fog Testing Period (ASTM B117), Mean Creepback Rating (ASTM D1654), Maximum Creepback Rating (ASTM D1654), Corrosion and Blisters (ASTM D1654). Multiple Paint samples are used in the evaluation of these tests and must meet the standards for a 1500 hour exposure to be considered a viable addition to the painting process. To evaluate the creep back and Corrosion tests a scribe must be inscribed into the coating and will be evaluated during its time while in the salt fog machine. The inspection intervals are conducted at 500 hours and 1000 hours up to the end of the test at 1500 hours. 
images before scribing procedure
File:Regular before Scribe.jpg|Base coating Before Scribing and salt fog testing
File:Therm before Crosshatch (Side A).jpg|Nano Ceramic additive added before scribing and salt fog
Scribed samples before salt fog test
File:Regular Scribe 2.jpg|standard base coating After scribing and Before salt fog testing 
File:ThermaCell Scribe 2.jpg|Nano Ceramic additive added after scribing and before salt fog testing
==MEK Standard==
This test technique is utilized to decide the level of fix of a heated film by the paint film protection from a predefined dissolvable. The Solvent Rub Test is generally performed utilizing methyl ethyl ketone (MEK) as the dissolvable. The MEK opposition or level of fix applies to paint topcoats and preliminaries. The paint coatings must meet the MEK Test (ASTM D4752-03) standard for 1500 hours. Methyl Ethyl Ketone (MEK) was rubbed on our samples, both the regular painted sample and the sample treated with a paint additive, to test to determine the level of resistance the paint surface film has against a specific solvent. The label for the sample with the paint additive applied is labeled as ThermaCell in order to match up with how the samples were labeled upon delivery. 
====Procedure==== 
1. Wipe clean the rub area on the sample to remove any residue with a dry cloth or cheesecloth and measure the sample thickness of the rub area with calipers. 
2. Mark with a sharpie a straight line to distinguish the two sides of which you will perform your MEK rub test. On one side of the line will be the before, and on the other side of the line will be the rub after the testing. 
3. Once your line is marked, take your dry cheesecloth and press down on the sample using. Apply pressure with one finger at a 45-degree angle and rub 50 times. One rub is considered a single there and back motion. 
4. After the 50 rubs, measure the thickness of the rub area on the sample. There should be no difference in thickness for the dry rub test. Rate the results of the rub based on a 1-5 scale provided by SEL. The characteristics of the ratings are 1 being the worst outcome and 5 having no effect on the surface and no paint on the cloth. 
5. Repeat this process with MEK dampened cheesecloth. Press down on the sample with the dampened section of cheesecloth. Apply pressure with one finger at a 45-degree angle and rub 50 times. One rub is considered a single there and back motion. 
6. Measure the thickness and rate your sample based on the 1-5 scale.
===Creepback Testing===
A typical test includes the intentional harm of the covering layer to decide a property alluded to as rust creep, a quantitative proportion of how far the consumption goes along the substrate/covering interface to one or the other side of a precisely actuated scratch during the introduction to a destructive climate—ordinarily an unbiased salt splash or cycle erosion test
==Cross-hatch adhesion test==
Each sample was scratched with the Elcometer 107 Crosshatch Cutter in order to create several parallel scratch marks ensuring the paint coating has bonded to the substrate. This test is performed by securing the sample in a vice and scratching it with the Crosshatch tool in a single, smooth motion. Two scratches will be made, one perpendicular to the other, creating a lattice cut where the scratches are intersecting. Three separate sites are created for each sample. Once the sites have been created, lightly brush off any loose debris and place a strip of Crosshatch Coating Adhesion Tape is laid on the intersection sites at a 45-degree angle to the intersection. Firmly press the tape on the site to ensure it has the most surface area contact with the scratch marks. Once firmly pressed on the surface, pull the tape off quickly revealing the lattice cut and making them available for analysis. This process was performed on our paint additive ThermaCell sample and the Regular painted sample and sent away to SEL for analysis.
===Scribing Instrumentation===
File:NVSCRIBETOOL.jpg|Scribing tool used to scratch surface coating
===crosshatch test imaging===
Standard Paint coating
File:Regular before Crosshatch.jpg|Standard paint coating before crosshatching
File:Reg Crosshatch Site 1.jpg|Standard paint coating After crosshatching 
Nanoceramic Paint additive added
File:Therm before Crosshatch (Side A).jpg|Nanoceramic additive added coating before crosshatching 
File:Therm Crosshatch Site 1.jpg|Nanoceramic additive added coating after crosshatching
==UV Testing==
Ultraviolet Exposure testing (UV testing) is going to be conducted on our coated coupons to understand how each respective coating will perform under the effects of ultraviolet exposure. With UV testing, we can simulate years of ultraviolet exposure in the time frame of a few days. With this test, we can evaluate the paint coatings for cracking, discoloration, and overall coating durability to UV rays.
==Nanoindentation==
Nanoindentation is a series of micro indentations on a substrate to characterize its material properties. We used this style of the test to characterize each respective paint coating and compare their values to the baseline coating. to begin the nanoindentation, the mounting plates that the samples were to be mounted to were cleaned in an ultrasonic cleaner. To mount each respective sample, We used double-sided tape to adhere to the mounts. The machine used tests the properties of the materials with the use of constant strain loading. In order to ensure the previous test didn't interfere with the next respective test space of 300 nanometers was given between each respective test and to account for the plastic deformation of the previous test. In order to ensure accuracy in our tests, we performed 25 tests on each respective coating. We decided to use a Poisson's ratio of .48 when conducting these tests which were similar to similar coatings of this style. We performed two separate rounds of testing with 1x1 coupons.
===Nanoindentation images===
File:NVNANOINDENTMACHINE.jpg|Nanoindentation Machine
File:NVNANOINDENTATIONSAMPLE.jpg|Nanoindentation sample of base coating
=Project Learning=
==Expected results==
*A vast array of temperature data in various climates
*Material properties of each respective coating
*data about the durability of each coating in various environments
*Thermal conductivity and resistivity information and models
*EMF protection information for each respective coating if time permits
==Phase Change Material (PCM) complications==
When this project was started the initial plan was going to be to test two paint additives with uniform testing and measurements. Once the PCM was shipped to our team we found that it was incompatible with the oil-based paint that was used for SEL's enclosures. (See Image Below)
File:PCM no mix.png|Pcm not mixing with oil based paint
In order to quantify the thermal properties of the PCM material we changed our focus and created separate enclosures. We then painted these enclosures with a water-based Sherman Williams paint and added the phase change material to one coating. In addition to static thermal testing, we also made an auxiliary heater circuit to further quantify the insulation properties of the PCM as well as the Nanoceramic coating.
=Results=
==SEM & optical microscope imaging==
To illustrate the surface texture and composition of each respective coating our team decided to employ the use of a scanning electron microscope (SEM) as well as an optical microscope. In order to accommodate a metallic coupon in the SEM we used carbon tape to ground the sample. With the use of microscopes, we were able to show the structure of the nanobeads as well as finding the average size of the beads in a respective sample. The Bead measurements can be found in the documents below.
With these images, we were able to find that the beads were randomly distributed and occupied from about 10-16% occupation of the sample. in addition, we found that the average diameter of the popped beads averaged 85 micrometers and the unpopped beads had an average diameter of 69.0625 micrometers. Our current hypothesis about the broken beads is that these broken beads don't provide as much thermal resistivity. 
===Dendritic Growths===
One interesting finding that we had when imaging both samples were the presence of Dendritic Growths on the paint surface. From our research, we have found that these growths are commonly found in most bridge paints. in this application, we think that these growths are reactions to surface contaminants on the base surface of the bare surface pre-paint. These growths are normally harder than the surface coating. Images of these dendritic growths can be seen below.
File:Thermalcell08.png
File:Thermalcell03.png
===EDS===
EDS stands for Energy Dispersive X-ray Spectroscopy. With this process, we were able to find the composition of the surface coating for all of our samples. the results can be found in the documents below.
EDS results
===Optical Microscope imaging===
To further characterize the surface texture and composition we used an optical microscope. This imaging allowed us to get a better idea about the dimensions for a larger majority of the surface. Some images can be seen below. 
File:50x Phase Change Material.jpg|Phase change material imaging
File:50X Nanoceramic.jpg|Nanoceramic material imaging
==Post Salt Fog Imaging==
In order to judge if the microstructure of the paint additive was damaged, our team took images after our environmental testing. The team took images of both the control and nanobead samples to provide the best comparison. Some images can be found below:
File:Regular05.jpg|Standard coating post salt fog
File:Regular06.jpg|Standard coating post salt fog alternate view
File:Thermocel.jpg|Nanobead coating post salt fog
File:Thermocelsecond.jpg|Nanobead coating post salt fog alternate view
comparing the images, we found that there was no major degredation to the nanobead coating. The number of intact beads was reduced from 77.42% of nanobead in a given area intact, to 65.56% intact nanoceramic beads. additional images of the samples can be found in the folder below.
Control coating post salt fog images
Nanobead coating post salt fog
===Bulk Images===
The bulk of the images can be found in the folders below.
SEM imaging
Optical microscope imaging
==MEK==
Regular Paint Sample: 
Thickness before MEK rub: 0.145 inch 
Thickness after MEK rub: 0.143 inch 
Resistance Rating: 3, minimal marring, some paint on cloth 
Paint Added Sample: 
Thickness before MEK rub: 0.145 inch 
Thickness after MEK rub: 0.145 inch 
Resistance Rating: 5, no effect on the surface, some paint on cloth but primarily from the sharpie mark 
===before MEK Testing===
File:Regular_before_Anything.jpg|No added paint additive sample before
File:ThermaCell before Anything.jpg|Nanoceramic particles added sample before
===After MEK Testing===
File:Reg after MEK.jpg|No added paint sample after MEK testd
File:Therm after MEK.jpg|NanoCeramic particles added sample after 
==Crosshatch adhesion test result==
We found that both coatings were within specification for the ASTM D2197
==Salt Fog Testing Results (1st Round of testing)==
===500 hour interval results===
the quantification began by vigorously using a spatula scraper tool and scraping the scribe mark indicated with the 500 hour mark at a 45 degree angle to determine paint wear on both the ThermaCell and Regular “ear” paint samples. Next, the samples were cleaned with water to rid of any debris caused by scraping. With the now cleaned samples, calipers were used to measure the width of the 500 hr scribe marks for both paint additives. scribe marks in six different locations along the line (ensuring at least an eighth of an inch from the endpoints). 
File:Samples after Scraping.jpg|Paint Additive samples after scraping
File:Regular.jpg|No Paint additive sample after scrape test
File:ThermaCell.jpg|Nano Ceramic additive sample after the scaping test
====initial observations====
Both samples had minimal paint loss, but the ThermaCell had slightly more than that of the regular sample when conducting the scraping using the spatula. an important note: The rust-colored substance is not actually rusted on these samples but rather a salt build-up
File:Samples before Scraping.jpg|Pre scrape samples at 500 hours of salt fog testing
====rust evaluation====
This is a visual test, and to determine rust evaluation both samples were flipped over (bottom side up without scribe marks) and evaluated within the central parts of the ear (away from edges or holes) to get the most accurate result. 
ThermaCell – score: 10 (0 rust) 
Regular – score: 10 (0 rust) 
====blistering====
This is a visual test to determine if there is any blistering in the paint. The test requires the same part of the sample as the rust evaluation. 
ThermaCell – score: 10 or “none” (no blistering) 
Regular – score: 10 or “none” (no blistering) 
====Creepback Results====
Creep back is determined by the equation below
C = (wc - w)/2 
C = creepage 
W_c = mean overall width of corrosion zone 
W = width of the original scribe mark 
*the variations in measurements are caused by user error due to the very small crack widths (hundredths of an inch) and the lack of a very precise measurement device for the required usage. Results can be found in the document below.
Creepback testing results 
===1000 hour test results===
Upon cleaning of both coupons, the regular sample had a little amount of flaking of paint. The ThermaCell, unfortunately, had a substantial chunk fail. The ThermaCell paint looks like it struggled to stay adhered to the metal surface. There was no blistering or rust on the backside of either paint sample except near the edges which we do not count.
File:20201229 095510.jpg|NanoCeramic coat results after 1000 hours
File:20201229 095520.jpg|Standard coat results after 1000 hours 
===1500 hour test results===
On the final interval of testing, we found that both the standard coating and the nano-ceramic coating had large chips in the paint. We think that the large chips were caused by the large circle on the mounting ear. In future testing, we will be using a uniform 4x6 coupon with a scribe stencil for more consistent testing.
File:1500 hour thermacell.jpg|1500 hour thermacell
File:1500 hour regular coat.jpg|1500 hour results on regular paint coat
==Salt Fog Testing results (Round Two)==
From our prior tests, we found that the Mounting ear sample was a bad sample to use for salt fog because of the proximity of the mounting ear circle to the scribe marks used to measure corrosion. To achieve reliable Data, Our team ran another series of salt fog tests on a proper rectangular sample. The images can be viewed below and the final tally of all measurements can be found in the results section.
===Initial Samples===
File:Regular w Scribes (1).jpg|Initial Regular Sample before the second Round of salt Fog testing
File:Thermacel w Scribes (1).jpg|Initial NanoBead Sample before the second round of salt Fog testing
===500 Hour Results===
File:Regular Front.jpg|500 hour standard coating results
File:Thermacell Front.jpg|500 hour results on thermacell paint coat
===1000 Hour Results===
File:Reg Front Pre-Scrape.jpg|1000 hour Standard coating pre scrape
File:Therm Front Pre-Scrape.jpg|1000 hour thermacell coating Pre scrape 
File:Reg Front Post-Scrape.jpg|1000 hour standard coating post scrape
File:Therm Front Post-Scrape.jpg|1000 hour thermacell coating post scrape
===Final Results ===
Our final results are indicated in the matrix below, In addition the mean and maximum creep can be seen in their respective charts below
File:Measurements.jpg|final salt fog measurements
File:Max Creepback.jpg|Maximum Creepback Graph
File:Mean Creepback.jpg|Mean creepback graph
===Conclusions===
From the salt fog testing, we found that the nano bead paint additive had no impact on the durability of the paint coating. this is supported by the final measurements of the scribe length along with the measurements for mean creep back and maximum creep back. These results also passed SEL's requirement for mean and max creep back and would allow for this paint additive to be implemented into their coating process.
==Nano Indentation Results==
===Round 1 testing===
The raw data can be found tabulated in the excel sheet below. The Minimum hardness factor found from the nanoindentation was a hardness of .122 GPA. The depth on the nanoindentation was limited to quantify solely the paint coating and not the substrate.
Nano Indentation Bulk Data
Nano Indentation Summary 
===Round 2 testing===
For this test, we compared two 1x1 coupons of each paint additive. Our tests indicated that the hardness of the Nanoceramic coating was lower at every average depth. in addition, there was a larger error indicated by the standard deviation of the mean. In the graph below, The bars represent the Standard deviation of the mean from the value
The bulk data can be found in the excel spreadsheets below
NanoIndentation bulk data second round (nanoceramic)
Nanoindentation Bulk Data Second round (standard coating)
===Hypothesis===
Our current working hypothesis on the smaller hardness levels has to do with the paint curing process. Due to the extra space that the nanobeads take up in the paint, we think they don't allow the paint to adhere to the base surface and cure effectively because of the space they take up in the paint.
===Round 3 testing (Post Salt fog testing)===
in order to further evaluate the integrity of the surface coating with the nanobead paint additive, Our team took measurements with nanoindentation of 1x1 samples before and after salt fog testing. We believe that by using the before and after comparison of the two samples we would be able to see if the nanobead particles degraded the surface integrity of the topcoating. The final samples after the enviormental testing can be in the images below.
File:1x1 Side By Side (Back).jpg|1x1 nanoindentation sample backside
File:1x1 Side By Side (Front).jpg|1x1 nanoindentation sample front face
The overall results with the pre and post salt fog samples can be seen in the graph below.
File:Nanoindentation final matrix.jpg|nanoindentation final results pre and post salt fog
We theorize that the salt from environmental testing added to the hardness values of each sample. however, the data still illustrates that there was no loss in the hardness of the coating with the nanoceramic additive embedded in it. The nanoindentation results are very promising and show that these nanoparticles could be implemented to SEL's Paint process and have no detriment to the integrity of the final paint coating
==Thermal Resistivity Results==
To analyze the thermal properties of each of the respective paint coating we started by taking temperature measurements on the outer surface of the cabinet along with the inside surface of the cabinet. With these temperature data points and their respective ΔT we were able to estimate the heat flux across the surfaces of the cabinet by estimating the thermal conductivity factor for the control cabinet with the standard coating. With this heat flux value, the respective thermal conductivity for the cabinets with the modified coating were collected and used to show heat transfer. 
Conduction equation: Q(w) = kA(Th - T∞) 
We found that the average thermal conductivity for a .2mm paint coating was about .2 w*m^-1*k^-1. With the primer and topcoat configuration of our coating system we estimated that our paint thickness was about .4mm which equates to a .4 w*m^-1K^-1 thermal conductivity of the paint for each side of the base material. With this, the total thermal conductivity addition to the base metal was estimated to be .8 w*m^-1K^-1. With these estimates in mind, we calculated the total thermal conductivity of the material to be 54.8 w*m^-1K^-1 for the base material. With this value, temperature data from 12/6/20 at 13:45 to find a base heat flux (q”) of 294.799 w*m^-1K^-1. By using this data in addition to the temperature delta information from the same date and found that the thermal conductivity value was found to be 52.2076 w*m^-1K^-1. With both thermal conductivity values found, the thermal resistivity values were found to be 0.000124136 K⋅m/W and.0001303 K⋅m/W for the control coating and ThermaCell coating respectively. This represents an increase of a little under 5% thermal resistivity between the two coatings.
==Temperature Testing Results==
One of the biggest aspects of this project was the temperature differential that this coating needed to provide. Our product requirements stated that the coating needed to provide a 5-degree increase above ambient temperatures in colder weather. On the other end of the spectrum, our coatings needed to provide a 5-degree drop in temperature in hotter weather climates. These requirements would allow for SEL to implement a lithium-ion battery into their enclosures which would reduce maintenance intervals and cost when compared to their current lead-acid battery. Our temperature data from December 6th, 2020 to January 3rd, 2021 can be found below. 
File:Screenshot20210307133606.jpg|frame|December 6th to January 3rd
Our current results show that in colder weather during the day, there is a two to three-degree increase from ambient. We are currently awaiting warmer temperatures to further quantify our coatings.
==Energy consumption and heater circuit results==
===Phase Change===
The final results for the insulative testing can be seen in the chart below:
File:Screenshot 2021-05-05 121210.jpg|Phase change insulative testing results
These results were found with our heater circuit. The way that these times were achieved was by counting the number of instances of the heater being on and converting it to seconds with the time between readings and adding for latency, This results in a reading every 1.152 seconds. With this information, we used the time on and the wattage rating of our heater to find energy usage in KWH. The final result was a 6.35% reduction in energy usage and a saving of almost two cents over the course of a week.
===NanoBead Testing===
We had taken some single day tests of the nanobead cabinets, however so far the results were inconclusive and more tests are being taken.
=External References=
Jung Yen Chou - Phase Change Materials.NW.2008
=Team Members=
	
Mark Currier
Major: Material Science And Engineering
Hometown: Snohomish, WA
Responsibility: Team Leader, SEM imaging
Email: curr8168@vandals.uidaho.edu		
Sara Beatty
Major: Material Science
Hometown: Issaquah, WA
Responsibility: Documentation Lead
Email: beat4576@vandals.uidaho.edu
	
Tyler Wallace
Major: Material science 
Hometown: Oakhurst, CA
Responsibility: SEM Imaging, 
Email: wall9454@vandals.uidaho.edu		
Cassidy Story
Major: Mechanical Engineering
Hometown: Sandpoint, ID
Responsibility: Budget Manager
Email: stor5666@vandals.uidaho.edu
	
Kyle Mays
Major: Mechanical Engineering
Hometown: Woodland Hills, CA
Responsibility: Wiki page manager, Thermal modeling lead, 
Email: Mays4003@vandals.uidaho.edu		
=Additional Documentation=
Meeting Minutes
*NanoTech Vandalizers Meeting minutes
Budget
*NanoTech Vandalizers Budget
Schedule
*NanoTech Vandalizers Gannt Chart
Snapshot Presentations
*NanoTech Vandalizers Snapshot 1
Concept Design Presentation
*NanoTech Vandalizers Concept Design Review